<p>After a lot of hard work and months of replacing and inspecting this issue I realized what's going on. The bowden tube gets soft as it gets hotter and hotter which allows the filament which is being extruded and retracted at a high speed to wear down the side of the tube. After some time the tube gets stretched out and it will eventually tear and that is seens as the hole in the pictures I provided. The solution to this problem is to upgrade to an all metal hotend, instate less aggressive retraction settings (which is what I did), or closely monitor your prints and replace your bowden tubing when it does eventually get  damaged (which I also do).</p>

CC BY-SA 4.0
2020-07-08T05:58:37.387Z
That may have sidestepped your problem but it's not "the solution" and has lots of tradeoffs. It sounds like the underlying problem was a fake Capricorn that's not even really PTFE.
R.. GitHub STOP HELPING ICE
CC BY-SA 4.0
2020-07-08T18:07:29.693Z
@R..GitHubSTOPHELPINGICE I'm afraid I purchased the Capricorn PTFE from Amazon  so I would assume it is real Capricorn tubing however, the detail about the PTFE getting soft as it gets hotter is information I got directly from Capricorns website so I am unsure as to why you think it's not real PTFE. I would like to point out that this kind of wear on the tubing is after hundreds of hours of printing so I am not sure what you mean by "lots of trade offs" I have found that less aggressive retraction has decreased my print times.
Daniel Bozarth
CC BY-SA 4.0
2020-07-08T19:29:13.250Z
That's why it's called a tradeoff. Faster prints, but wrong extrusion (material oozed in wrong place) leading to weak and ugly parts. Other tradeoffs too.
R.. GitHub STOP HELPING ICE
CC BY-SA 4.0
2020-07-09T18:49:48.007Z
You assume that there is material oozing but there is no such thing. I assure you I never said that  I was getting weak and ugly parts after this solution. I would appreciate it if you could elaborate on these other trade-offs because this solution I presented is working quite well for me and the 20 machines I run it on.
Daniel Bozarth
CC BY-SA 4.0
2020-07-07T16:16:34.930Z
2020-07-07T16:16:34.930Z
Daniel Bozarth
<p>If the tube is PTFE, the tube is not likely to be melting unless your hotend temperature is out of control.  You would probably notice the PLA cooking.</p>

<p>So, perhaps they aren't PTFE, or perhaps it is wear.</p>

<p>If it wasn't PTFE, you should be able to tell by the texture, slipperiness, and bending force.</p>

<p>The four thinned faces look like they would correspond to four of the barbs in the connector.  The thinned ring below the four thinned faces look like a wear line where the tube is pressing against the exit of the connector.  It looks to me as if the tube is moving or flexing in the connector.  The barbs act as little chisels cutting into the tube, which is how they restrain such a slippery material as PTFE.</p>

<p>It might work better if the tube were a little longer.  This might reduce the forces at the limits of movement which may be placing strain on the tubes.  If you can, you might also fashion a strain relief for the tube so that it doesn't bend right as it exist from the connector. If you can cut down on the movement, you will help with the external wear.</p>

<p>It is also possible that the tubes are being strained by a high filament pressure.  All the drive to push filament into the hot end is matched by an equivalent reverse pressure from the tube onto the connector.  If you can stand a higher print temperature, the life of the tube may be increased.</p>

<p>@towe added a comment:</p>

<blockquote>
  <p>I don't think those are marks from the teeth of the pneumatic coupler. The questions states "where it pushes against the nozzle", and the Ender 3 Pro seems to have a hot-end where the Bowden tube reaches all the way through the cold end and heat break to the nozzle.</p>
</blockquote>

<p>A mechanical drawing of what may be a MK-10 hot-end as used on the Ender 3 Pro also suggests that the Ender 3 Pro has a PTFE lined hot end.  Lets accept that drawing as confirming that @towe is right.  Never-the-less, the marks you show in the photo look like the types of cuts I have seen from a pneumatic coupler.  How can we reconcile this contradiction?</p>

<p>The most direct answer would be that the tube is not reaching through to the nozzle.  In the photo you don't show enough of the blue tube to show the coupler scars which should be a little further up the tube.  Suppose that, in fact, the tube is not pressing against the nozzle.  This might not be the case if any of these are true:</p>

<ol>
<li>There is a separate piece of PTFE that is permanently in hot end. 
The Creality Ender 3 Pro looks as if
it is not configured for a Bowden feed.  A PTFE lined hot-end for a
direct extruder would have a piece of PTFE cut to length in the
hot-end.  A simple mod to make that a Bowden would leave that
sculpted PTFE tube in place.</li>
<li>The pneumatic couplers have been replaced.  Many couplers do not
permit the tube to pass through them, although the hole in the end
can be drilled to 4mm diameter.  In fact, preventing the tube from
passing through a pneumatic coupler is a feature in the intended
application of coupling to air tubes in moderate pressure
applications.</li>
<li>There is a bump in the path that is catching the  tube and
preventing it from extending through to the cold end and onward.</li>
</ol>

CC BY-SA 4.0
2020-02-20T12:17:41.640Z
I don't think those are marks from the teeth of the pneumatic coupler. The questions states "where it pushes against the nozzle", and the Ender 3 Pro seems to have a hotend where the bowden tube reaches all the way through the cold end and heat break to the nozzle.
towe
CC BY-SA 4.0
2020-02-20T14:52:18.503Z
@towe, Thank you for your comment.  With your encouragement, I looked deeper and added more information to my answer.
cmm
CC BY-SA 4.0
2020-02-21T23:56:21.020Z
I am afraid those marks are not from the pneumatic coupler, the gouges from the coupler are hidden just out of view by my thumb. I would take another picture and show you however I threw the piece away already. I know that the tube reaches all the way to the nozzle as there was no filament attached to the end of the tube which would happen as the filament approaches the nozzle and clogs any space between the nozzle and the tube end.
Daniel Bozarth
CC BY-SA 4.0
2020-02-22T01:31:28.380Z
The Ender 3 Pro is designed with Bowden tube feeding in mind, it is a stock feature and there is one only one continuous tube from the extruder driver to the butt of the nozzle. The pneumatic couplers have been replaced but they are the type to allow tubing to pass through them.
Daniel Bozarth
CC BY-SA 4.0
2020-02-22T03:54:01.173Z
@Daniel a remaining possibility,  unbolt though it seems to me, is that the tubes are melting.   If so they aren't suitable for the job.   When you have another failure, please take lots of close up pictures.   You could also try a melt test on the tube.   Put it in a 300°C oven for a couple of hours and check for any change or softening.   Maybe put a clip on it and see if the tube collapses.
cmm
CC BY-SA 4.0
2020-02-19T20:59:09.877Z
2020-02-20T14:44:41.790Z
2020-02-20T14:44:41.790Z
cmm
<p>This isn't melting, it is wear.</p>
<p>And it isn't typical wear you would expect due to abrasion.   It is wear caused by retraction.   As your filament retracts (usually between parts of the model to reduce stringing), the semi-molten filament is sucked back into the tube.</p>
<p>Then, when the filament is unretracted, the filament is pushed back into the nozzle.   However, in the meantime, a little of the filament solidified on the PTFE wall.   PTFE is very slippery, so the solidified chunk is peeled off the wall no problems - but it takes with it a tiny bit of the inside of the tube.</p>
<p>Do that hundreds of thousands of times, and the wall of the tube gets thinned at that point until it fails.</p>
<p>One solution to this is to reduce retraction.   Notice how the distance between the worn bit and the end of the tube is always the retraction distance in millimeters?</p>
<p>Another solution is an all metal hotend.</p>
<p>Or just trim your bowden tube shorter by a few mm every hundred hours of printing or so.</p>

CC BY-SA 4.0
2023-03-09T18:23:07.930Z
2023-03-09T18:23:07.930Z
Oliver Mattos
<p>I run a 3D printer farm and I have to replace my Bowden tubes on the printers after about a month or two of use(roughly 1000 hours of use). The Bowden tubes continually melt on the side of the tube very near to where it pushes against the nozzle. I am running Ender 3 Pros and I run at about 205&nbsp;&deg;C with PLA. The Bowden tubes I have are some I found on Amazon and they are not Capricorn tubes. </p>

<p><a href="https://i.sstatic.net/xnhmZ.png" rel="nofollow noreferrer"><img src="https://i.sstatic.net/xnhmZ.png" alt="Note how the hole is very near the base of the tube closest to the nozzle"></a></p>

<p>EDIT1: I have added more pictures below of a new failure. This time you can see the marks of the teeth of the coupler a good inch below the failure point.
<a href="https://i.sstatic.net/QPk6E.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/QPk6E.jpg" alt="New photo of tube 1"></a>
<a href="https://i.sstatic.net/A3xXQ.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/A3xXQ.jpg" alt="New photo of tube 2"></a>
<a href="https://i.sstatic.net/P9l5a.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/P9l5a.jpg" alt="New photo of tube 3"></a>
<a href="https://i.sstatic.net/PB7Ox.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/PB7Ox.jpg" alt="New potho of tube 4"></a></p>

CC BY-SA 4.0
2020-02-19T18:44:43.273Z
Melting is virtually impossible, that happens at 327 °C. To me this looks more like wear.
0scar
CC BY-SA 4.0
2020-02-19T18:48:34.767Z
Hmm, so you're saying that wear caused a tear in the tube?
Daniel Bozarth
CC BY-SA 4.0
2020-02-19T18:51:37.210Z
I'm saying that it cannot be melting caused by heat of printing PLA :) It *looks* as if it is wear. What other failure modes are possible?
0scar
<creality-ender-3><bowden>
What causes my Bowden tube to melt on the side?
Daniel Bozarth
# What causes my Bowden tube to melt on the side?

(Asked by: username_0 on 2020-02-19)

I run a 3D printer farm and I have to replace my Bowden tubes on the printers after about a month or two of use(roughly 1000 hours of use). The Bowden tubes continually melt on the side of the tube very near to where it pushes against the nozzle. I am running Ender 3 Pros and I run at about 205 °C with PLA. The Bowden tubes I have are some I found on Amazon and they are not Capricorn tubes.

[![Note how the hole is very near the base of the tube closest to the nozzle](https://i.sstatic.net/xnhmZ.png)](https://i.sstatic.net/xnhmZ.png)

EDIT1: I have added more pictures below of a new failure. This time you can see the marks of the teeth of the coupler a good inch below the failure point.
[![New photo of tube 1](https://i.sstatic.net/QPk6E.jpg)](https://i.sstatic.net/QPk6E.jpg)
[![New photo of tube 2](https://i.sstatic.net/A3xXQ.jpg)](https://i.sstatic.net/A3xXQ.jpg)
[![New photo of tube 3](https://i.sstatic.net/P9l5a.jpg)](https://i.sstatic.net/P9l5a.jpg)
[![New potho of tube 4](https://i.sstatic.net/PB7Ox.jpg)](https://i.sstatic.net/PB7Ox.jpg)

**Tags:** creality-ender-3, bowden
> **Comments:**
> **username_1**: Melting is virtually impossible, that happens at 327 °C. To me this looks more like wear.  
> **username_0**: Hmm, so you're saying that wear caused a tear in the tube?  
> **username_1**: I'm saying that it cannot be melting caused by heat of printing PLA :) It *looks* as if it is wear. What other failure modes are possible?  

---

## 3 answers

### Answer by username_0 on 2020-07-07. Score: 1 | Accepted answer

After a lot of hard work and months of replacing and inspecting this issue I realized what's going on. The bowden tube gets soft as it gets hotter and hotter which allows the filament which is being extruded and retracted at a high speed to wear down the side of the tube. After some time the tube gets stretched out and it will eventually tear and that is seens as the hole in the pictures I provided. The solution to this problem is to upgrade to an all metal hotend, instate less aggressive retraction settings (which is what I did), or closely monitor your prints and replace your bowden tubing when it does eventually get damaged (which I also do).

> **Comments:**
> **username_2**: That may have sidestepped your problem but it's not "the solution" and has lots of tradeoffs. It sounds like the underlying problem was a fake Capricorn that's not even really PTFE.  
> **username_0**: @R..GitHubSTOPHELPINGICE I'm afraid I purchased the Capricorn PTFE from Amazon  so I would assume it is real Capricorn tubing however, the detail about the PTFE getting soft as it gets hotter is information I got directly from Capricorns website so I am unsure as to why you think it's not real PTFE. I would like to point out that this kind of wear on the tubing is after hundreds of hours of printing so I am not sure what you mean by "lots of trade offs" I have found that less aggressive retraction has decreased my print times.  
> **username_2**: That's why it's called a tradeoff. Faster prints, but wrong extrusion (material oozed in wrong place) leading to weak and ugly parts. Other tradeoffs too.  
> **username_0**: You assume that there is material oozing but there is no such thing. I assure you I never said that  I was getting weak and ugly parts after this solution. I would appreciate it if you could elaborate on these other trade-offs because this solution I presented is working quite well for me and the 20 machines I run it on.  

---

### Answer by username_3 on 2020-02-19. Score: 2

If the tube is PTFE, the tube is not likely to be melting unless your hotend temperature is out of control. You would probably notice the PLA cooking.

So, perhaps they aren't PTFE, or perhaps it is wear.

If it wasn't PTFE, you should be able to tell by the texture, slipperiness, and bending force.

The four thinned faces look like they would correspond to four of the barbs in the connector. The thinned ring below the four thinned faces look like a wear line where the tube is pressing against the exit of the connector. It looks to me as if the tube is moving or flexing in the connector. The barbs act as little chisels cutting into the tube, which is how they restrain such a slippery material as PTFE.

It might work better if the tube were a little longer. This might reduce the forces at the limits of movement which may be placing strain on the tubes. If you can, you might also fashion a strain relief for the tube so that it doesn't bend right as it exist from the connector. If you can cut down on the movement, you will help with the external wear.

It is also possible that the tubes are being strained by a high filament pressure. All the drive to push filament into the hot end is matched by an equivalent reverse pressure from the tube onto the connector. If you can stand a higher print temperature, the life of the tube may be increased.

@towe added a comment:

> I don't think those are marks from the teeth of the pneumatic coupler. The questions states "where it pushes against the nozzle", and the Ender 3 Pro seems to have a hot-end where the Bowden tube reaches all the way through the cold end and heat break to the nozzle.

A mechanical drawing of what may be a MK-10 hot-end as used on the Ender 3 Pro also suggests that the Ender 3 Pro has a PTFE lined hot end. Lets accept that drawing as confirming that @towe is right. Never-the-less, the marks you show in the photo look like the types of cuts I have seen from a pneumatic coupler. How can we reconcile this contradiction?

The most direct answer would be that the tube is not reaching through to the nozzle. In the photo you don't show enough of the blue tube to show the coupler scars which should be a little further up the tube. Suppose that, in fact, the tube is not pressing against the nozzle. This might not be the case if any of these are true:

1. There is a separate piece of PTFE that is permanently in hot end.
   The Creality Ender 3 Pro looks as if
   it is not configured for a Bowden feed. A PTFE lined hot-end for a
   direct extruder would have a piece of PTFE cut to length in the
   hot-end. A simple mod to make that a Bowden would leave that
   sculpted PTFE tube in place.
2. The pneumatic couplers have been replaced. Many couplers do not
   permit the tube to pass through them, although the hole in the end
   can be drilled to 4mm diameter. In fact, preventing the tube from
   passing through a pneumatic coupler is a feature in the intended
   application of coupling to air tubes in moderate pressure
   applications.
3. There is a bump in the path that is catching the tube and
   preventing it from extending through to the cold end and onward.

> **Comments:**
> **username_4**: I don't think those are marks from the teeth of the pneumatic coupler. The questions states "where it pushes against the nozzle", and the Ender 3 Pro seems to have a hotend where the bowden tube reaches all the way through the cold end and heat break to the nozzle.  
> **username_3**: @towe, Thank you for your comment.  With your encouragement, I looked deeper and added more information to my answer.  
> **username_0**: I am afraid those marks are not from the pneumatic coupler, the gouges from the coupler are hidden just out of view by my thumb. I would take another picture and show you however I threw the piece away already. I know that the tube reaches all the way to the nozzle as there was no filament attached to the end of the tube which would happen as the filament approaches the nozzle and clogs any space between the nozzle and the tube end.  
> **username_0**: The Ender 3 Pro is designed with Bowden tube feeding in mind, it is a stock feature and there is one only one continuous tube from the extruder driver to the butt of the nozzle. The pneumatic couplers have been replaced but they are the type to allow tubing to pass through them.  
> **username_3**: @Daniel a remaining possibility,  unbolt though it seems to me, is that the tubes are melting.   If so they aren't suitable for the job.   When you have another failure, please take lots of close up pictures.   You could also try a melt test on the tube.   Put it in a 300°C oven for a couple of hours and check for any change or softening.   Maybe put a clip on it and see if the tube collapses.  

---

### Answer by username_5 on 2023-03-09. Score: 0

This isn't melting, it is wear.

And it isn't typical wear you would expect due to abrasion. It is wear caused by retraction. As your filament retracts (usually between parts of the model to reduce stringing), the semi-molten filament is sucked back into the tube.

Then, when the filament is unretracted, the filament is pushed back into the nozzle. However, in the meantime, a little of the filament solidified on the PTFE wall. PTFE is very slippery, so the solidified chunk is peeled off the wall no problems - but it takes with it a tiny bit of the inside of the tube.

Do that hundreds of thousands of times, and the wall of the tube gets thinned at that point until it fails.

One solution to this is to reduce retraction. Notice how the distance between the worn bit and the end of the tube is always the retraction distance in millimeters?

Another solution is an all metal hotend.

Or just trim your bowden tube shorter by a few mm every hundred hours of printing or so.


---

